Growth of few-wall carbon nanotubes with narrow diameter distribution over Fe-Mo-MgO catalyst by methane/acetylene catalytic decomposition
- Vladimir A Labunov†1Email author,
- Alexander S Basaev2,
- Boris G Shulitski1,
- Yuriy P Shaman†1, 2,
- Ivan Komissarov1,
- Alena L Prudnikava1Email author,
- Beng Kang Tay3 and
- Maziar Shakerzadeh3
© Labunov et al; licensee Springer. 2012
Received: 6 December 2011
Accepted: 2 February 2012
Published: 2 February 2012
Few-wall carbon nanotubes were synthesized by methane/acetylene decomposition over bimetallic Fe-Mo catalyst with MgO (1:8:40) support at the temperature of 900°C. No calcinations and reduction pretreatments were applied to the catalytic powder. The transmission electron microscopy investigation showed that the synthesized carbon nanotubes [CNTs] have high purity and narrow diameter distribution. Raman spectrum showed that the ratio of G to D band line intensities of IG/ID is approximately 10, and the peaks in the low frequency range were attributed to the radial breathing mode corresponding to the nanotubes of small diameters. Thermogravimetric analysis data indicated no amorphous carbon phases. Experiments conducted at higher gas pressures showed the increase of CNT yield up to 83%. Mössbauer spectroscopy, magnetization measurements, X-ray diffraction, high-resolution transmission electron microscopy, and electron diffraction were employed to evaluate the nature of catalyst particles.
Carbon nanotubes [CNTs] due to their incredible properties have attracted scientific and practical interest for almost 20 years . High electrical and thermal conductance, striking mechanical strength, and an especially unique chirality-dependence electronic structure make CNTs one of the most promising alternatives to replace some of today's materials used in microelectronics manufacturing. In particular, due to an enormous field enhancement factor and high conductivity, CNTs are perfect sources for electron emission . Tremendous numbers of attempts have been made to use carbon nanotube arrays as the field-emission cathodes [FECs] . Single-wall carbon nanotubes [SWNT] provide a large field enhancement factor, low threshold voltage, and high emission currents, but the substantial degradation of emission currents is a serious bottleneck for the application of SWNT-based FECs . In contrast, multi-wall carbon nanotubes [MWNTs] have high emission stability but have a small field enhancement factor. Few-wall carbon nanotubes [FWNTs] are considered as an ideal choice for this application . Despite the progress in producing high-impurity and high-yield few-wall CNTs , the cost and simplicity of CNT fabrication still remain as the major problems limiting their wide application. In general, the main methods of CNT synthesis are arc discharge, pulsed laser ablation, and chemical vapor deposition [CVD]. CVD method has been recognized as the most suitable for commercial production of CNTs. The use of large specific surface powder with catalytic sites distributed on it is the common approach for high-yield CNT processes. Fabrication of a catalyst for synthesis of CNTs with desired geometrical properties (number of walls) is the art of today's carbon nanotube technology.
So far, bimetallic catalysts are accepted as the most efficient for high-yield production of CNTs. Metal alloys such as Co-Ni , Fe-Co [8, 9], Fe-Mo [6, 10], and Co-Mo [11, 12] were utilized in catalysts for CNT growth. There are a number of works discussing the transition metals: molybdenum ratio and role of molybdenum in the efficient growth of CNTs with uniform diameter distribution [13–16]. A high amount of molybdenum in Fe-Mo alloy leads to the growth of larger-diameter CNTs, and vice versa, decreasing the Mo content in bimetallic alloy favors smaller-diameter CNT synthesis. This fact most likely relates to the catalytic particle size dependence on FexMoyOz phases from which these particles are released during the reduction process; in turn, oxide phase formation depends on calcination (annealing) processes .
Usually, hydrogen serves as a reduction agent for catalyst activation. Variation of hydrogen flow during the reduction step and hydrogen/hydrocarbon ratio during the synthesis affects the quality and purity of the CNT product . On the other hand, transition metal catalysts themselves are known as promoters of methane decomposition for high-rate hydrogen conversion . It allows us to avoid the use of any additional reducing agent for catalyst activation.
Simplification of the high-yield production method and reducing the cost of catalyst components are two crucial steps towards the commercialization of the FWNT product. In this paper, we describe the developed technological approach for a simple and efficient FWNT synthesis.
Finally, the catalyst was placed in a quartz boat and then directly loaded into the hot zone of a 15-mm tubular furnace at the temperature of 900°C while the furnace was purged with 100 cm3/min of Ar. When the temperature was stable, 40 cm3/min flow of methane was introduced. After 15 min, the CH4 flow was set to zero simultaneously introducing 10 cm3/min of acetylene flow. The CNT growth process was stopped by switching off the C2H2 flow, and the product was immediately removed from the hot zone and cooled down to the room temperature at 300 cm3/min of Ar flow which took about 5 min. The synthesis of CNTs at higher pressure was performed at the same conditions described above except that after 45 min of the process, the gas pressure was increased up to 2 bars and the process continued additionally for 20 min.
Various techniques were employed in order to characterize the prepared CNTs. Raman spectroscopy was performed using the Renishaw spectrometer with a laser wavelength of 514 nm (Renishaw, Wotton-under-Edge, UK). A JEOL 2010 transmission electron microscope (JEOL Ltd., Akishima, Tokyo, Japan) operated at 200 kV was used to study the microstructure. A DRON-3M X-ray diffractometer with CuK source was employed to collect X-ray diffraction [XRD] spectra (Bourevestnik Inc., St. Petersburg, Russia). The Mössbauer spectra were collected in transmission geometry at room temperature using the MS2000 spectrometer with 57Fe/Rh source (40 mCu) (Belarusian State University, Minsk, Belarus). Magnetization of synthesized CNTs was measured by a ponderomotive method . Calorimetric measurements were performed with a Mettler-Toledo instrument TGA/DSC-1/1600 HF (Mettler-Toledo, Inc., Greifensee, Switzerland) setup in dry air flow and at a heating rate of 1°C/min.
There are few peaks in the range below 300 cm-1 in the Raman spectrum. Commonly, peaks in this range are assigned to the radial breathing mode [RBM] of SWCNTs. Using the simple inverse relation v = 9 +235/d (where ν is the frequency in units of inverse centimeter, d is diameter of nanotubes in nanometers), we estimated the diameters of the nanotubes in the range of 0.9 to 1.7 nm; the larger diameters cannot be estimated from the spectrum because of the spectrometer frequency cutoff. Besides, these peaks in the range below 300 cm-1, apart from the RBM mode of SWNTs, can be attributed to the RBM mode of the inner tubes of FWNTs .
As we pointed in the introduction part, the simple and cheap technology for producing CNTs with desired geometry of carbon nanotubes opens the way to a wide range of applications of CNTs. We would like to emphasize that our technological approach does not contain any additional calcinations or reduction step after the catalyst preparation. Besides, catalyst preparation process is consuming a lot less time; the elimination of a calcination step prevents the large-size catalytic particle formation, thus limiting the diameter distribution of CNTs in the final product. Although iron nanoparticles are initially in the oxide state, the presence of methane partially reduces the oxides, which leads to the enhancement of the methane decomposition by the presence of metal particles. Bimetallic catalysts show better methane decomposition performance, and the decomposition rate depends on the Fe/Mo ratio . In our work the Fe/Mo ratio is optimized for few-wall nanotube synthesis.
Moreover, it was revealed that reaction with methane not only reduces the iron oxide to iron, but also turns some fraction of it into cementite , which is reported to be not catalytically active for methane/acetylene decomposition . From the magnetic measurement data and Mössbauer spectrum, we conclude that most of the nanoparticles are in Fe3C phase in the final product. Only the selected area electron diffraction data indicated the presence of some amount of γ-Fe phase. We do believe that some part of cementite observed by our ex-situ measurements was formed during the cooling process when carbon interacting with the γ-Fe particles transited to the cementite phase .
Growth of CNTs is considered as a multistep process involving formation of Fe3C from iron catalyst nanoparticles [26–28]. Formation of CNTs from cementite was demonstrated by in-situ TEM measurements . However, there are still debates whether Fe3C could promote formation and growth of very thin CNTs . In general, catalytic activity and carbon solubility of catalytic species depend on the temperature, diffusion, and particle size. Thus, catalyst species could be active or inactive depending on the carbon atom kinetics. Molybdenum, due to the higher carbon solubility as compared to iron , can serve as a regulator of carbon atom kinetics for neighboring γ-Fe and Fe3C catalyst species, preventing their poisoning at the conditions we perform our synthesis. The Fe2MoC phase observed using HRTEM in our experiment claimed to be inactive for CNT growth . That phase most probably arises from the FexMoyOz phase, and its formation is limited due to the absence of calcination. The low amount of Fe2MoC can be explained this way (Mössbauer and XRD spectra do not show any evidence of this phase).
Let us briefly discuss the impact of synthesis pressure on CNT yield. It was revealed that prolongation of reaction time in our experiments for more than 45 min did not increase significantly the mass of the CNT product. That fact usually contributed to the diffusion issue of carbon feedstock molecules through the mat of CNTs . However, it was found that increasing the pressure up to 2 bars in the furnace during CNT synthesis, as was described in the experimental part, leads to the CNT-yield increase approximately by 20 wt.% (see Figure 9, red curve). Thus, we attribute the longer catalytic activity and, as a consequence, the higher CNT yield at the realized synthesis conditions to the increasing hydrocarbon molecular diffusivity as the gas pressure increases.
The technological approach for the simple high-yield CVD growth of few-wall carbon nanotubes was developed. The Fe-Mo-MgO catalyst with 1:8:40 molar ratio was prepared by impregnation method from purum quality components without any calcinations and reduction steps. TEM, Raman, and thermogravimetrical studies showed that decomposition of methane/acetylene at 900°C over the catalyst leads to the formation of CNTs with diameters in the range of 2 to 10 nm. The phase of catalytic species in CNT was investigated by ex-situ Mössbauer, XRD, HRTEM, and electron diffraction techniques. The phase transitions of metallic components of binary catalyst and their role in the CNT growth process were discussed. It was demonstrated that slightly increasing the gas pressure during the CNT growth leads to the increase in the CNT yield.
chemical vapor deposition
differential scanning calorimetry
few-wall carbon nanotube
high-resolution transmission electron microscopy
multi-wall carbon nanotube
single-wall carbon nanotube
transmission electron microscopy
The authors would like to thank J. A. Fedotova for the Mössbauer spectroscopy measurements and data analysis and K.I. Yanushkevich for the X-ray diffraction and magnetization measurements.
- Iijima S: Helical microtubules of graphitic carbon. Nature 1991, 354: 56–58. 10.1038/354056a0View ArticleGoogle Scholar
- Saito Y, Uemura S: Field emission from carbon nanotubes and its application to electron sources. Carbon 2000, 38: 169–182. 10.1016/S0008-6223(99)00139-6View ArticleGoogle Scholar
- Anantram M, L'eonard F: Physics of carbon nanotube electronic devices. Rep Prog Phys 2006, 69: 507–561. 10.1088/0034-4885/69/3/R01View ArticleGoogle Scholar
- Uemura S, Yotani J, Nagasako T, Kurachi H, Yamada H, Ezaki T, Maesoba T, Maesoba T, Nakao T, Saito Y, Yumura M: Large size FED with carbon nanotube emitter. SID 02 DIGEST 2002, 33: 1132–1135. 10.1889/1.1830144View ArticleGoogle Scholar
- Pan ZW, Au FCK, Lai HL, Zhou WY, Sun LF, Liu ZQ, Tang DS, Lee CS, Lee ST, Xie SS: Very low-field emission from aligned and opened carbon nanotube arrays. J Phys Chem B 2001, 105: 1519–15226. 10.1021/jp0033824View ArticleGoogle Scholar
- Jeong HJ, Kim KK, Jeong SY, Park MH, Yang CW, Lee YH: High-yield catalytic synthesis of thin multiwalled carbon nanotubes. J Phys Chem B 2004, 108: 17695–17698. 10.1021/jp046152oView ArticleGoogle Scholar
- Singh BK, Ryu H: The effect of Ni-Co catalyst composition on the yield and nanostructure of carbon nanofibers synthesized by CVD. Solid State Phenom 2007, 119: 227–230.View ArticleGoogle Scholar
- Maruyama S, Kojima R, Miyauchi Y, Chiashi S, Kohno M: Low-temperature synthesis of high-purity single-walled carbon nanotubes from alchohol. Chem Phys Lett 2002, 360: 229–234. 10.1016/S0009-2614(02)00838-2View ArticleGoogle Scholar
- Murakami Y, Miyauchi Y, Chiashi S, Maruyama S: Characterization of single-walled carbon nanotubes catalytically synthesized from alcohol. Chem Phys Lett 2003, 374: 53–58. 10.1016/S0009-2614(03)00687-0View ArticleGoogle Scholar
- Li Y, Liu J, Wang Y, Wang ZL: Preparation of monodispersed Fe-Mo nanoparticles as the catalyst for CVD synthesis of carbon nanotubes. Chem Mat 2001, 13: 1008–1014. 10.1021/cm000787sView ArticleGoogle Scholar
- Tang S, Zhong Z, Xiong Z, Sun L, Liu L, Lin J, Shen ZX, Tan KL: Controlled growth of single-walled carbon nanotubes by catalytic decomposition of CH4over Mo/Co/MgO. Chem Phys Lett 2001, 350: 19–26. 10.1016/S0009-2614(01)01183-6View ArticleGoogle Scholar
- Kitiyanan B, Alvarez WE, Harwell JH, Resasco DE: Controlled production of single-wall carbon nanotbes by catalytic decomposition of CO on bimetallic Co-Mo catalysts. Chem Phys Lett 2000, 317: 497–503. 10.1016/S0009-2614(99)01379-2View ArticleGoogle Scholar
- Liao XZ, Serquis A, Jia QX, Peterson DE, Zhu YT, Xu HF: Effect of catalyst composition on carbon nanotube growth. Appl Phys Lett 2003, 82: 2694–2696. 10.1063/1.1569655View ArticleGoogle Scholar
- Pérez-Mendoza M, Vallés C, Maser WK, Martínez MT, Benito AM: Influence of molybdenum on the chemical vapour deposition production of carbon nanotubes. Nanotechnology 2005, 16: 224–229. 10.1088/0957-4484/16/5/016View ArticleGoogle Scholar
- Curtarolo S, Awasthi N, Setyawan W, Jiang A, Bolton K, Tokune T, Harutyunyan AR: Influence of Mo on the Fe:Mo:C nanocatalyst thermodynamics for single-walled carbon nanotube growth. Phys Rev B 2008., 78(5): http://prb.aps.org/abstract/PRB/v78/i5/e054105 http://prb.aps.org/abstract/PRB/v78/i5/e054105
- Yoshida H, Shimizu T, Uchiyama T, Kohno H, Homma Y, Takeda S: Atomic-scale analysis on the role of molybdenum in iron-catalyzed carbon nanotube growth. Nano Lett 2009, 9: 3810–3815. 10.1021/nl9019903View ArticleGoogle Scholar
- Lamouroux E, Serp P, Kihn Y, Kalck P: Identification of key parameters for the selective growth of single or double wall carbon nanotubes on FeMo/Al2O3 CVD catalysts. Appl Catalysis A 2007, 323: 162–173. http://www.sciencedirect.com/science/article/pii/S0926860X07000993 http://www.sciencedirect.com/science/article/pii/S0926860X07000993View ArticleGoogle Scholar
- Xiong GY, Suda Y, Wang DZ, Huang JY, Ren ZF: Effect of temperature, pressure, and gas ratio of methane to hydrogen on the synthesis of double-walled carbon nanotubes by chemical vapour deposition. Nanotechnology 2005, 16: 532–535. 10.1088/0957-4484/16/4/033View ArticleGoogle Scholar
- Shah N, Panjala D, Huffman GP: Hydrogen production by catalytic decomposition of methane. Energy Fuels 2001, 15: 1528–1534. 10.1021/ef0101964View ArticleGoogle Scholar
- Chechernikov VI: Magnetic Measurements. Moscow: Moscow State University; 1969.Google Scholar
- Kim DY, Yang CM, Park YS, Kim KK, Jeong SY, Han JH, Lee YH: Characterization of thin multi-walled carbon nanotubes synthesized by catalytic chemical vapor deposition. Chem Phys Lett 2005, 413: 135–141. 10.1016/j.cplett.2005.07.064View ArticleGoogle Scholar
- Ajayan PM, Ebbesen TW, Ichihashi T, Iijima S, Tanigaki K, Hiura H: Opening carbon nanotubes with oxygen and implications for filling. Nature 1993, 362: 522–525. http://www.sciencedirect.com/science/article/pii/S037838200300064X http://www.sciencedirect.com/science/article/pii/S037838200300064X 10.1038/362522a0View ArticleGoogle Scholar
- Shah N, Pattanaik S, Huggins FE, Panjala D, Huffman GP: XAFS and Mössbauer spectroscopy characterization of supported binary catalysts for nonoxidative dehydrogenation of methane. Fuel Proc Tech 2003, 83: 163–173. 10.1016/S0378-3820(03)00064-XView ArticleGoogle Scholar
- Takaneka S, Serizawa M, Otsuka K: Formation of filamentous carbons over supported Fe catalysts through methane decomposition. J of Catalysis 2004, 222: 520–531. 10.1016/j.jcat.2003.11.017View ArticleGoogle Scholar
- Prudnikava AL, Fedotova JA, Kasiuk JV, Shulitski BG, Labunov VA: Mössbauer spectroscopy investigation of magnetic nanoparticles incorporated into carbon nanotubes obtained by the injection CVD method. Sem Phys Quan Elect & Opt 2010, 13: 125–131. http://www.nbuv.gov.ua/PORTAL/natural/SQO/2010_2/v13n2–2010-p125–131.pdf http://www.nbuv.gov.ua/PORTAL/natural/SQO/2010_2/v13n2-2010-p125-131.pdfGoogle Scholar
- Jost O, Gorbunov AA, Möller J, Pompe W, Liu X, Georgi P, Dunsch L, Golden MS, Fink J: Rate-limiting processes in the formation of single-wall carbon nanotubes: pointing the way to the nanotube formation mechanism. J Phys Chem B 2002, 106: 2875–2883. 10.1021/jp013138sView ArticleGoogle Scholar
- Stadermann M, Sherlock SP, In JB, Fornasiero F, Park HG, Artyukhin AB, Wang Y, De Yoreo JJ, Grigoropoulos CP, Bakajin O, Chernov AA, Noy A: Mechanism and kinetics of growth termination in controlled chemical vapor deposition growth of multiwall carbon nanotube arrays. Nano Lett 2009, 9: 738–744. 10.1021/nl803277gView ArticleGoogle Scholar
- Esconjauregui S, Whelan CM, Maex K: The reasons why metals catalyze the nucleation and growth of carbon nanotubes and other carbon nanomorphologies. Carbon 2009, 47: 659–669. 10.1016/j.carbon.2008.10.047View ArticleGoogle Scholar
- Yoshida H, Takeda S, Uchiyama T, Kohno H, Homma Y: Atomic-scale in-situ observation of carbon nanotube growth from solid state iron carbide nanoparticles. Nano Lett 2008, 8: 2082–2086. 10.1021/nl080452qView ArticleGoogle Scholar
- Kulikov IS: Termodinamika Karbidov i Nitridov (Thermodynamics of Carbides and Nitrides). Chelyabinsk: Metallurgija; 1988:149–152.Google Scholar
- Hafner JH, Bronikowski MJ, Azamian BR, Nikolaev P, Rinzler AG, Colbert DT, Smith KA, Smalley RE: Catalytic growth of single-wall carbon nanotubes from metal particles. Chem Phys Lett 1998, 296: 195–202. 10.1016/S0009-2614(98)01024-0View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.